Structure and phase transitions of LiTaOGeO~4~
Malcherek, Thomas; Acta Crystallographica Section B 58 (2002) 607–612; doi:10.1107/S010876810200825X

data_2103315
_publ_section_title
;
 Structure and phase transitions of LiTaOGeO~4~
;
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              607
_journal_page_last               612
_journal_paper_doi               10.1107/S010876810200825X
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ge Li O5 Ta'
_chemical_formula_weight         340.48
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 119.5450(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   7.57730(10)
_cell_length_b                   8.11880(10)
_cell_length_c                   7.49100(10)
_cell_measurement_reflns_used    164
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      44.7
_cell_measurement_theta_min      8.7
_cell_volume                     400.913(9)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_method       'omega-2theta scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0230
_diffrn_reflns_av_sigmaI/netI    0.0242
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            1809
_diffrn_reflns_theta_full        34.87
_diffrn_reflns_theta_max         34.87
_diffrn_reflns_theta_min         3.98
_exptl_absorpt_coefficient_mu    34.666
_exptl_absorpt_correction_T_max  0.3450
_exptl_absorpt_correction_T_min  0.0705
_exptl_absorpt_correction_type   numerical
_exptl_crystal_density_diffrn    5.641
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             592
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.04
_refine_diff_density_max         1.939
_refine_diff_density_min         -2.430
_refine_ls_extinction_coef       0.0367(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.036
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     40
_refine_ls_number_reflns         877
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.036
_refine_ls_R_factor_all          0.0202
_refine_ls_R_factor_gt           0.0158
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0213P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0356
_refine_ls_wR_factor_ref         0.0370
_reflns_number_gt                776
_reflns_number_total             877
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ck0010.cif
_cod_data_source_block           ltgo_amb_split
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               2103315
_cod_database_fobs_code          2103315